# Timoshenko beam model for buckling of piezoelectric nanowires with surface effects

- Arash Tourki Samaei
^{1, 2}Email author, - Majid Bakhtiari
^{2}and - Gang-Feng Wang
^{3}

**7**:201

**DOI: **10.1186/1556-276X-7-201

© Samaei et al; licensee Springer. 2012

**Received: **13 October 2011

**Accepted: **27 March 2012

**Published: **27 March 2012

## Abstract

This paper investigates the buckling behavior of piezoelectric nanowires under distributed transverse loading, within the framework of the Timoshenko beam theory, and in the presence of surface effects. Analytical relations are given for the critical force of axial buckling of nanowires by accounting for the effects of surface elasticity, residual surface tension, and transverse shear deformation. Through an example, it is shown that the critical electric potential of buckling depends on both the surface stresses and piezoelectricity. This study may be helpful in the characterization of the mechanical properties of nanowires and in the calibration of the nanowire-based force sensors.

### Keywords

surface elasticity buckling piezoelectric nanowire## Introduction

Nanowires have attracted considerable attention in the literature for future applications as sensors, actuators, transistors, and resonators in nanoelectromechanical systems and in biotechnology [1]. Because of these varied applications, it is very important to accurately characterize the mechanical properties of nanowires and their response to external loading. In atomistic scales, owing to the increasing ratio of surface area to volume, the stress and strain effects on surface physics become very important [2]. In this regard, theoretical and experimental investigations have provided a better understanding of the effects of stress on surface physics [3, 4]. For example, by conducting bending tests using atomic force microscopy, Cuenot et al. [4] have demonstrated that the stiffness of nanowires is size-dependent, and this phenomenon has been theoretically explained by considering the surface effects [5–8]. He and Lilley [6] investigated the influences of surface tension on the static bending of nanowires. Wang and Feng [8] studied the surface effects on the buckling and vibration behaviors of nanowires, based on the Laplace-Young equation. The theoretical investigations related to the surface effects and mechanical behavior show a good agreement with the experiments and atomistic simulations [3, 6, 9].

Recently, piezoelectric nanostructures, such as nanowires, have been drawing a lot of attention due to their potential applications as nanoresonators [10], diodes [11], and nanogenerators [12]. Piezoelectric nanomaterials exhibit size-dependent properties at nanoscale, and also, it has been demonstrated that they have larger piezoelectric constants than their bulk counterparts [13, 14]. Experimental measurements and atomistic simulations demonstrate that the elastic and fracture properties of ZnO piezoelectric nanowires vary with their cross-sectional dimensions [5, 15, 16]. Zhao et al. [17] found out that the effective piezoelectric coefficient of the ZnO nanowire is frequency-dependent and that it is much larger than that of the bulk material. Using the perturbation theory [13] and finite element method [14], the electrostatic potential in a bending piezoelectric nanowire was calculated. For the first time, Wang and Feng [18] used the Euler-Bernoulli beam model to investigate the buckling and vibration behaviors of piezoelectric nanowires by taking into account the effects of surface stresses and piezoelectricity. Also, surface effects and surface piezoelectricity are considered to study the electromechanical coupling behavior of piezoelectric nanowires with the Euler beam theory by Yan and Jiang [19].

The objective of the present paper is to investigate the combined surface and piezoelectric effects on the buckling of piezoelectric nanowires using the modified Timoshenko beam model. In this study, the two modified Euler beam and Timoshenko beam models have been compared, but no quantitative experimental measurement has been reported on the buckling condition of piezoelectric nanowires. A numerical example is presented in the article to demonstrate both the surface and piezoelectric effects, and then, some discussions are provided based on the obtained results.

## Formulation of the problem

*l*, width

*b*, and height 2

*h*, as shown in Figure 1. The mechanical properties of the bulk part (

*E*,

*G*, and

*ρ*) designate the Young's modulus, shear modulus, and mass density of the nanowire, respectively.

In the current study, a crystalline ZnO nanowire with the C_{6v} symmetry about the poling direction along the *z*-axis [18] is considered, which has a surface layer with surface elasticity modulus (*E*^{5}) [20–22], which can be determined by atomistic simulations or experiments [3, 23], surface layer thickness (*t*) [8], and constant residual surface tension (*τ*^{0}) [18, 24]. The effect of the residual surface stress acting as a transverse load on the nanowire is calculated by the Laplace-Young equations [25].

*γ*(

*J*/

*m*

^{2}) to Young's modulus

*E*(

*J*/

*m*

^{3}),

*γ*/

*E*, leads to some intrinsic length scale material parameter in the nanometer range [26, 27]. When a material element has a characteristic length comparable to the intrinsic scale, the surface/interface energy can play an important role in its properties and behavior. According to Gibbs [26], the surface stress tensor ${\sigma}_{\alpha \beta}^{\mathsf{\text{5}}}$ is related to the surface energy density

*γ*as follows:

^{2}

*w*/∂

*x*

^{2}, where

*w*is the deflection at the position

*x*[29]. For the current study, the electric field is assumed to exist in the

*z*direction. For the one-dimensional piezoelectric nanowire, the strain and stress can be obtained as follows [30]:

*c*

_{22},

*e*

_{32}, and

*ψ*are the linear elastic constant, the linear piezoelectric coefficient, and the electric potential of the piezoelectric material, respectively, and ${\gamma}^{0}=\frac{\partial w}{\partial x}-\varphi $ is the shear strain. For the piezoelectric nanowire, the electric displacements with the applied strain and electric field for the piezoelectric nanowire can be written as follows [30]:

*λ*

_{11}and

*λ*

_{33}are the dielectric constants. The electric field component is

*E*

_{ x }≪

*E*

_{ z }because the electric potential is almost constant along the nanowire (

*x*-axis) except around the two ends [13]. Using the electrostatic equilibrium condition, the electric potential can be obtained [18], and thus, the stress of the piezoelectric nanowire can be calculated. For the hinged-hinged piezoelectric nanowire, a resultant axial force (

*T*

_{ x }) is induced by the applied electric potential as follows [18]:

*A*and

*κ*are the cross-sectional area and the shear correction factor of the cross section, respectively. Generally, the shear correction factor is considered to be in the range of 0.833 ≤

*κ*

^{2}≤ 0.870. Since the applied electric potential may induce a compressive axial force due to piezoelectric effects, it is essential to determine the critical electric potential for the buckling of piezoelectric nanowires. Solving Equation 7 for the hinged-hinged nanowire, the critical electric potential corresponding to the buckling of the noted nanowire can be obtained as follows:

where *ξ* is the slenderness ratio (slenderness ratio corresponds to length-to-the least radius of gyration of the cross section ratio) of the nanowire, and for a hinged-hinged beam, *ξ* = 1 [8]. Equation 8 presents a relation between the residual surface stress of a piezoelectric nanowire and the critical electric potential in the buckling analysis. Therefore, it can be inferred that the elasticity modulus and the residual surface stress could be obtained by measuring the critical electric potentials of two nanowires with different sizes [18].

## Example and discussion

*c*

_{11}= 207 Gpa,

*e*

_{31}= -0.51 C/m

^{2}, and

*λ*

_{33}= -7.88 × 10

^{-11}F/m [18], and its surface energy density on the (0001)-plane is

*γ*= 1.6 J/m

^{2}[30]. The formulations in the 'Formulation of the problem' section indicate that the buckling behavior of piezoelectric nanowires largely depends on their surface and piezoelectric properties, which could be determined either by experiments or atomistic simulations [3, 6, 28, 30]. For example, Miller and Shenoy [3] determined the free surface properties of aluminum using the embedded atom method for some crystallographic directions. By neglecting the shear deformation effect in Equation 8, the Euler model with surface effects is obtained [18] as follows:

It is found from Equation 8 that the shear deformation lowers the critical compression force of buckling in comparison with the classical Euler solution.

*Vcr*/

*Vcr*0) has been plotted versus the nanowire height (

*h*) in Figure 2. Here,

*Vcr*0 is the critical electric potential for the buckling obtained from the Euler model without the surface effects. Figure 2 has been plotted for the first mode of buckling and also for several aspect ratios. By observing the curves, it can be concluded that, contrary to the classical model, the normalized critical electric potential depends on a size characteristic such as the nanowire height. These curves show that by reducing the nanowire height to the sub-20-nm range, both the surface and piezoelectric effects become more and more influential. Moreover, as the nanowire height increases, the curves converge and ultimately turn into those of the classical case, pointing out the fact that with the increase of the nanowire height, the surface effects are eliminated. On the other hand, it is seen that the normalized critical electric potential obtained from the modified Timoshenko beam model is smaller than that obtained from the modified Euler beam model, which shows that, in order to get more exact results, both the surface and shear deformation effects should be taken into consideration.

In this study, the thickness of the surface layer has been disregarded because it is very small relative to the sizes of the nanowire's geometrical parameters. Also, in the present investigation, the assumption is that the deformation of the nanowire is small and that the resultant principle (the principle of superposition) can be used to sum up the tensions arising from the surface and piezoelectric effects; therefore, the effect of surface tension has been modeled as a curvature-dependent transverse loading, and the piezoelectric effect has been modeled as an induced axial force in the nanowire.

## Conclusion

In the present study, by applying the modified Timoshenko beam theory and considering the effects of surface, piezoelectricity, and shear deformation, the buckling behavior of piezoelectric nanowires was investigated. The obtained information can be used in the design and characterization of piezoelectric nanowire-based devices and instruments. The critical electric potential for the buckling of piezoelectric nanowires with the hinged-hinged boundary condition was derived analytically. The results show that, in addition to the surface effects, the shear deformation and piezoelectricity can effectively influence the buckling behavior of nanowires as well. Also, it was observed that, contrary to the surface effects, the shear deformation tends to reduce the critical electric potential and that it has a greater influence on stubby nanowires with smaller aspect ratios. Therefore, for smaller nanowire heights in the nanometer range, the effects of surface elasticity, piezoelectricity, and shear deformation should be taken into consideration so that more accurate results are obtained.

## Declarations

## Authors’ Affiliations

## References

- Zhong Z, Wang D, Cui Y, Bockrath MW, Lieber CM: Nanowire crossbar arrays as address decoders for integrated nanosystems.
*Science*2003, 302: 1377–1379. 10.1126/science.1090899View Article - Wang GF, Li XD: Predicting the Young's modulus of nanowires from first-principles calculations on their surface and bulk materials.
*J Appl Phys*2008, 104: 113517. 10.1063/1.3033634View Article - Miller RE, Shenoy VB: Size-dependent elastic properties of nanosized structural elements.
*Nanotechnology*2000, 11: 139–147. 10.1088/0957-4484/11/3/301View Article - Cuenot S, Frétigny C, Demoustier-Champagne S, Nysten B: Surface tension effect on the mechanical properties of nanomaterials measured by atomic force microscopy.
*Phys Rev B*2004, 69: 165410.View Article - Chen CQ, Shi Y, Zhang YS, Zhu J, Yan YJ: Size dependence of Young's modulus in ZnO nanowires.
*Phys Rev Lett*2006, 96: 075505.View Article - He J, Lilley CM: Surface effect on the elastic behavior of static bending nanowires.
*Nano Lett*2008, 8: 1798. 10.1021/nl0733233View Article - Wang GF, Feng XQ: Surface effects on buckling of nanowires under uniaxial compression.
*Appl Phys Lett*2009, 94: 141913. 10.1063/1.3117505View Article - Wang GF, Feng XQ: Timoshenko beam model for buckling and vibration of nanowires with surface effects.
*J Phys D Appl Phys*2009, 42: 155411. 10.1088/0022-3727/42/15/155411View Article - Gavan KB, Westra HJR, van der Drift EWJM, Venstra WJ, van der Zant HSJ: Size-dependent effective Young's modulus of silicon nitride cantilevers.
*Appl Phys Lett*2009, 94: 233108. 10.1063/1.3152772View Article - Bai XD, Gao PX, Wang ZL, Wang EG: Dual-mode mechanical resonance of individual ZnO nanobelts.
*Appl Phys Lett*2003, 82: 4806–4808. 10.1063/1.1587878View Article - He JH, Hsin CL, Liu J, Chen LJ, Wang ZL: Piezoelectric gated diode of a single ZnO nanowire.
*Adv Mater*2007, 19: 781–784. 10.1002/adma.200601908View Article - Wang ZL, Song JH: Piezoelectric nanogenerators based on zinc oxide nanowires.
*Science*2006, 312: 242. 10.1126/science.1124005View Article - Xiang HJ, Yang JL, Hou JG, Zhu QS: Piezoelectricity in ZnO nanowires: a first-principles study.
*Appl Phys Lett*2006, 89: 223111. 10.1063/1.2397013View Article - Li C, Guo WL, Kong Y, Gao HJ: Size-dependent piezoelectricity in zinc oxide nanofilms from first-principles calculations.
*Appl Phys Lett*2007, 90: 033108. 10.1063/1.2430686View Article - Agrawal R, Peng B, Gdoutos EE, Espinosa HD: Elasticity size effects in ZnO nanowires-a combined experimental-computational approach.
*Nano Lett*2008, 8: 3668. 10.1021/nl801724bView Article - Agrawal R, Peng B, Espinosa HD: Experimental-computational investigation of ZnO nanowires strength and fracture.
*Nano Lett*2009, 9: 4177. 10.1021/nl9023885View Article - Zhao MH, Wang ZL, Mao SX: Piezoelectric characterization of individual zinc oxide nanobelt probed by piezoresponse force microscope.
*Nano Lett*2004, 4: 587–590. 10.1021/nl035198aView Article - Wang GF, Feng XQ: Effect of surface stresses on the vibration and buckling of piezoelectric nanowires.
*EPL*2008, 91: 56007.View Article - Yan Z, Jiang L: Surface effects on the electromechanical coupling and bending behaviours of piezoelectric nanowires.
*J Phys D: Appl Phys*2011, 44: 075404. 10.1088/0022-3727/44/7/075404View Article - Gurtin ME, Markenscoff X, Thurston RN: Effect of surface stress on the natural frequency of thin crystals.
*Appl Phys Lett*1976, 29: 529. 10.1063/1.89173View Article - Wang GF, Feng XQ: Effects of surface stresses on contact problems at nanoscale.
*J Appl Phys*2007, 101: 013510. 10.1063/1.2405127View Article - Wang GF, Wang TJ, Feng XQ: Surface effects on the diffraction of plane compressional waves by a nanosized circular hole.
*Appl Phys Lett*2006, 89: 231923. 10.1063/1.2403899View Article - Jing GY, Duan HL, Sun XM, Zhang ZS, Xu J, Li YD, Wang JX, Yu DP: Surface effects on elastic properties of silver nanowires: contact atomic-force microscopy.
*Phys Rev B*2006, 73: 235409.View Article - Wang GF, Feng XQ: Effects of surface elasticity and residual surface tension on the natural frequency of microbeams.
*Appl Phys Lett*2007, 90: 231904. 10.1063/1.2746950View Article - Chen T, Chiu MS, Weng CN: Derivation of the generalized Young-Laplace equation of curved interfaces in nanoscaled solids.
*J Appl Phys*2006, 100: 074308. 10.1063/1.2356094View Article - Gibbs JW:
*The Scientific Papers of J Willard Gibbs, Vol. 1: Thermodynamics*. New York: Longmans and Green; 1906. - Cammarata RC: Surface and interface stress effects in thin films.
*Prog Surf Sci*1994, 46: 1.View Article - Shenoy VB: Atomistic calculations of elastic properties of metallic fcc crystal surfaces.
*Phys Rev B*2005, 71: 094104.View Article - Rao SS:
*Vibration of Continuous Systems*. New Jersey: Wiley; 2007. - Gao YF, Wang ZL: Electrostatic potential in a bent piezoelectric nanowires. The fundamental theory of nanogenerator and nanopiezotronics.
*Nano Lett*2007, 7: 2499. 10.1021/nl071310jView Article

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.